26 2.3 Recombination

Table 2.4: Relaxation Regimes after Photoexcitation. The four temporally-overlapping relaxation
regimes following an initial photoexcitation with an ultrashort laser pulse in a semiconductor.^{120}The listed
time scale and respective interactions for each regime describe the path of an excited electron in the CB
back to its initial position in the VB.

𝑡 =0.0 ps excitation: “e-h pair generation”

• absorption of incident ultrashort fs-pulse

• electron transition “VB to CB”

𝑡 ≤0.2 ps coherent regime:“time until first collision”

• momentum scattering

• carrier-carrier scattering

• intervalley scattering

𝑡 ≤2 ps non-thermal regime:“equilibrium among carriers”

• carrier-carrier scattering

• intervalley scattering

• carrier-optical phonon scattering

𝑡 ≤100 ps hot-excitation regime:“equilibrium with the lattice”

• hot-carrier-phonon scattering

• decay of optical phonons

• carrier-acoustic phonon scattering 50 ps≤ 𝑡 isothermal regime: “e-h pair recombination”

• carrier recombination

• electron transition “CB to VB”

Both the non-thermal and the hot-excitation regimes mainly involve scattering processes through
which excited electrons relax towards the CBM. These interactions and their temporal decay have
been studied extensively by my former colleague Dr. Verena Hintermayr within bulk and 2D LHP
nanoplatelets.^{52,121}Therefore, time-resolved studies of these effects are not included in this thesis,
however, the interaction with phonons will be examined as a cause for spectral broadening of
transi-tions.

The reverse process to absorption — in a sense that electrons and holes recombine — finally takes place in the so-called isothermal regime. Recombination will represent the main focus of the remainder of this section and will hence be explained in greater detail in the following subsection.

As a final remark it shall be noted that e-h pairs can diffuse within the crystal or even to adjacent NCs before their recombination. Longer lifetimes of e-h pairs enhance the probability for these processes.

Moreover, even charge extraction after e-h pair dissociation may occur at an interface with an adjacent material. This will be examined inChapter 6, while the respective theoretical background will be laid out inSection 2.5.

28 2.3 Recombination 2.3.2 Radiative and Nonradiative Recombination

Generally, e-h recombination either occurs via a radiative or a nonradiative mechanism. All of the interband relaxation paths observed in the context of the present work may be assigned to one of three different categories which will be highlighted below. For the description of these processes one needs to distinguish between the recombination of free e-h pairs and that of excitons.

Radiative Recombination

### a b

E

one-particle picture two-particle picture

2s continuum 1s

E

k K

CB

VB electron

hole

### }

excitonω1

ω2

Figure 2.8: Radiative Recombination. (a)Radiative recombination of free e-h pairs mainly occurs at the relaxed state (“CBM to VBM”). Thereby an excited electron falls back into the VB and a photon with the respective energy is emitted.(b)The two-particle picture is needed to represent the same context for excitons.

As the name suggests, this type of recombination involves the emission of photons, resulting in photoluminescence (PL). Consequently, this is the sought-after process within LHP NCs that are destined for efficient light emission. More details on PL and its efficiency will be explained in Subsection 3.3.3. Here, this effect is solely introduced and compared to the respective nonradiative mechanisms.

Figure 2.8 ashows the process of radiative recombination for free e-h pairs in the so-called one-particle picture based on a schematic illustration of the electronic band structure around the direct band gap.

Here, the electron and hole are highlighted as red and white circles in the CB and VB, respectively.

Usually, intraband relaxation to the CBM or VBM is a much faster process compared to interband
recombination. Therefore, most instances of the latter process mainly involve electrons that relax
from the CBM to the VBM as illustrated in the scheme for the direct band gap of LHPs. Due to the
negligible change in momentum compared to the energy difference, such transitions are drawn as
vertical lines. In this process, the electron transfers the resulting energy difference to a photon that
is consequently emitted. In contrast, the energy levels of excitons cannot be represented using the
one-particle picture. Instead, the two-particle picture must be applied, which illustrates the excitonic
states with respect to the continuum (seeFigure 2.8 b).^{56}In this picture, radiative recombination may
only occur along the linear dispersion function of light, which is indicated by the grey dashed line
in the scheme. This process is similar to free e-h recombination, however, it experiences different
dynamics and exhibits the emission of a slightly red-shifted photon compared to the other process.

Trap-Assisted Recombination

E

one-particle picture

k

CB

VB electron trap

Figure 2.9: Trap-assisted Recombination. This scheme illustrates the nonradiative monomolecular process which involves the capture of an electron (or hole) into a specific trap state.

Subsection 2.2.2already introduced the term “defect tolerance” as a property of LHPs. Trap states in
LHPs are usually located close to the edge of energy bands or even within them.^{82}Moreover, many
defects exhibit a shallow character, meaning that the thermal energy of electrons is sufficient for them
to leave the trap. Still, these traps open up relaxation channels, leading to nonradiative recombination
via phonon interactions. The respective scheme for this mechanism is shown inFigure 2.9. For
excitons this is more complex and cannot be depicted properly, yet the effect itself also exists for
bound e-h pairs.

Auger Recombination and Exciton-Exciton Annihilation

### a b

E

one-particle picture two-particle picture

2s continuum 1s

E

k K

CB1

VB electron

hole

### }

exciton CB2Figure 2.10: Auger Recombination and Exciton-Exciton Annihilation. (a)At least three particles are involved in higher-order Auger processes. In the course of its interband transition to the VB, the energy of an electron is transferred to another electron in the CB which is lifted to a higher conduction band CB2 in response. Via interaction with phonons, it could end up at a higher energy on the same band CB1, as well. Note that, conversely, the reverse process is possible for holes in the VB.(b)The counterpart interaction for excitons in the two-particle picture is the so-call exciton-exciton annihilation. While falling back to the ground state, an exciton transfers its energy to another nearby exciton which is thereby lifted into the continuum.

30 2.3 Recombination In all recombination processes, energy and momentum conservation must be satisfied. While both mechanisms introduced so far rely on an energy transfer to a photon or to phonons, respectively, we finally turn to another effect in which energy is transferred to another carrier (electron, hole or exciton).

This phenomenon is referred to as Auger recombination for free e-h pairs and as exciton-exciton
annihilation for excitons. Free e-h pairs may also transfer their energy to another nearby electron in
the CB or a hole in the VB instead of emitting a photon via radiative recombination. This third charge
carrier is promoted into an energetically higher band, while the other two free charge carriers are
annihilated. Of course, and as depicted inFigure 2.10 a, this is a three-particle process. It may therefore
only be observed for sufficiently high charge carrier densities.^{122}Again, the two-particle picture is
needed to explain the related process for excitons (seeFigure 2.10 b). In exciton-exciton annihilation,
the released energy of an exciton is transferred to another exciton.^{123}Usually, this energy exceeds the
exciton binding energy𝐸_{B}, such that the exciton absorbing this energy is lifted into the continuum
where it persists as a free e-h pair. However, via the aforementioned fast intraband relaxation channels,
this free e-h pair often quickly relaxes back to its original excitonic state via phonon scattering. The
exciton-exciton annihilation process in thin LHP nanoplatelets is studied within this work. Therefore,
this effect shall be discussed in greater detail in the following subsection.

2.3.3 Exciton-Exciton Annihilation

As mentioned above, exciton-exciton annihilation is a nonradiative multiparticle process known to be
strongly dependent on the excitation density since increased exciton densities enhance the probability
for such events to occur.^{123,124}With this in mind and only referring to excitons, the process of
exciton-exciton annihilation represents the exact opposite to so-called monomolecular exciton-exciton recombination
in which only a single exciton recombines either radiatively emitting a photon or nonradiatively via
traps. Therefore, exciton-exciton annihilation needs to be considered one of the limiting factors for
luminescent LHP NCs. A purpose of this work was to understand how this mechanism is affected by
the size of NCs. Nanoplatelets (NPls) with variable thickness in the confined dimension are a suitable
material for this purpose and were accordingly utilized as samples. These confined systems exhibit
high exciton binding energies much smaller than the thermal energy of electrons. Therefore, we could
assume for our experiments conducted at room temperature that all excited e-h pairs exist as excitons
after a fast initial intraband relaxation.^{20}

exciton-exciton annihilation

monomolecular recombination

τ4 τ3 τ2

τ1

τ1 τ1 τ1

Figure 2.11: Scheme of an Interband Relaxation Pathway for a Single Nanoplatelet.A single NPl
initially containing four excitons predominantly undergoes exciton-exciton annihilation processes until
only one exciton remains. Due to the higher exciton density, the annihilation processes described by
the lifetimes𝜏_{4}and𝜏_{3}occur even faster than those described by𝜏_{2}. During the first tens of picoseconds
monomolecular recombination (𝜏_{1}) plays a negligible role as indicated by the thin arrows.

First, the possible recombination processes shall only be illustrated for one single NPl. This is shown inFigure 2.11where the initial photoexcitation led to the generation of four excitons within the NPl.

From this starting point, the exciton population may either decay via exciton-exciton annihilation (𝜏_{4},
𝜏_{3},𝜏_{2}) or via monomolecular recombination (𝜏_{1}). As reported by Klimov et al., recombination rates are
quantized within small NCs, such that the resulting recombination rate of an individual NPl depends
on the exact amount of excitons the respective NPl contains.^{123}Generally, the relaxation from𝑁to
𝑁 − 1excitons slows down with decreasing𝑁as the carrier density within the equally sized NPls is
accordingly reduced. For the population decay shown inFigure 2.11, this means that the lifetimes
increase gradually, i.e.,𝜏_{4}< 𝜏_{3}< 𝜏_{2} < 𝜏_{1}. In the colloidal CdSe NCs studied by Klimov et al.,𝜏_{2}turned
out to be more than one order of magnitude smaller than𝜏_{1}. Here, I already want to reveal, that this
difference in magnitude between𝜏_{2}and𝜏_{1}even surpasses two orders of magnitude for the case of the
CsPbBr_{3}NPls studied in this thesis. Due to this drastic difference, the process described by𝜏_{2}occurs at
a much faster timescale and, therefore, it is a reasonable assumption that exciton-exciton annihilation
is the dominant recombination process for all NPls containing more than one exciton. This is also the
reason why the less likely monomolecular recombination process is indicated by thinner arrows in
Figure 2.11.

On this basis, the actual exciton-exciton annihilation experiment shall be explained. As already stated inSubsection 2.2.3the experiments within this thesis are not conducted on single NCs as illustrated in Figure 2.11. Therefore, in the next step, an ensemble of many NPls has to be considered. Regarding the model used to analyze the experiment, it is important that excitons in different NPls of the illuminated ensemble do not interact with each other. In particular, excitons within a distinct NPl should not have the possibility to transfer to a nearby NPl. Therefore, the NPls were dispersed in hexane, such that no NPl had direct contact to other NPls due to their low concentration within the cuvette.

Against this backdrop,Figure 2.12describes how exciton-exciton annihilation processes can be observed
experimentally. Initially, all NPls are in thermal equilibrium and no NPl contains excitons (the amount
of thermally excited charge carriers can be neglected). An ultrashort laser pulse excites an ensemble
of NPls promoting electrons from the VB to the CB, thereby initially creating free e-h pairs. The
subsequent intraband relaxation processes within these thin 2D structures occur so fast that already
after around 1 ps all excited e-h pairs can be assumed to have formed excitons. This situation is defined
as𝑡 = 0in the scheme ofFigure 2.12. The yellow panel illustrates that some NPls of the ensemble do
not contain any exciton, whereas other NPls may possess several. In fact, those are the ones of interest
for the process of exciton-exciton annihilation since at least two excitons are needed within a single
NPl to observe this effect. This annihilation between excitons happens on a short time scale, such that
it can be assumed that after several tens of picoseconds all of the NPls initially containing more than
one exciton, reduce this amount to exactly one remaining exciton (cf. “𝑡 = 𝑡_{1}” inFigure 2.12). Then,
slower monomolecular recombination becomes the dominant process with lifetimes in the nanosecond
regime. The cycle of this experimental scheme repeats itself only once every 2 ms, starting with the
next excitation pulse. Due to this long pause it can be assumed that thermal equilibrium — i.e., a state
with no excitons in the NPls (cf. “𝑡 = 𝑡_{2}” inFigure 2.12) — is reached easily each time before the next
excitation pulse arrives on the sample.

32 2.3 Recombination exciton-exciton

annihilation

ultrafast

excitation monomolecular

recombination

t = 0 t = t1

t = t2

~ fs

~ ps

~ ns

Figure 2.12: Time Sequence of the Exciton-Exciton Annihilation Experiment.Initially, excitation
is caused using an ultrashort laser pulse. Already after∼1 ps, all of the excited e-h pairs relax down to the
exciton level, establishing a Poisson distribution over the observed NPls (𝑡 = 0, which — by exception — does
not define the exact moment of the excitation here, but the moment approximately 1 ps thereafter).
Exciton-exciton annihilation with lifetimes in the low ps-regime is a much faster process compared to Exciton-excitonic
or trap-assisted recombination. Therefore, it may be assumed that all of the exciton-exciton annihilation
processes occur before monomolecular recombination — involving only one exciton per NPl — becomes
the dominant contribution to the overall interband relaxation process (𝑡 = 𝑡_{1}). The latter mechanism takes
place within several nanoseconds after, while the ultrafast excitation is only initiated once every 2 ms.

Therefore, it is a safe assumption that no NPl contains an exciton before the next excitation-relaxation
cycle starts (𝑡 = 𝑡_{2}).

In order to describe exciton-exciton annihilation mathematically, the following definitions shall be introduced:

𝑛_{total}=^{∧}“total number of observed NPls”

𝑁_{total}=^{∧}“total number of excitons at𝑡 = 0”

𝑁=^{∧}“number of excitons within an individual NPl at𝑡 = 0”

𝑛(𝑁 )=^{∧}“number of NPls with N excitons at𝑡 = 0”

⟨𝑁 ⟩ = 𝑁_{total}/𝑛total=^{∧}“average number of excitons per NPl at𝑡 = 0”

(2.34)

An exemplary set of these values can be extracted fromFigure 2.12, from which one obtains𝑛_{total} = 8,
𝑁_{total} = 14, and⟨𝑁 ⟩ = 1.75. Furthermore, there are three NPls containing exactly two excitons at𝑡 = 0,

translating to𝑛(𝑁 = 2) = 3. Adding up all NPls in groups like this with the same amount of excitons will always yield the total number of NPls, i.e.,

𝑁_{total}

∑

𝑁 =0

𝑛(𝑁 ) = 𝑛_{total}. (2.35)

N = 0 N ≥ 3

N = 1

N = 2

0 0.2 1.0

0.0 0.4 0.6 0.8

1 2 3 4 5

P(

〈N〉

〈N〉, N)

Figure 2.13: Poisson Distribution.At𝑡 = 0, excitons are distributed across all observed NPls according
to Poisson statistics. In the experiment, the average number of excitons per NPl⟨𝑁 ⟩is controlled via the
pump power which determines how many photons arrive at the excitation volume that contains a fixed
number of observed NPls𝑛_{total}.Equation 2.36is plotted here as a function of⟨𝑁 ⟩for the cases𝑁 = 0,𝑁 = 1,
𝑁 = 2, and𝑁 ≥ 3. This way, for a fixed⟨𝑁 ⟩, one may look up the percentage of NPls that contain zero,
one, two, or more NPls at𝑡 = 0, respectively.

While this holds true in general, we can be more precise for the mentioned experiment. The excitons
generated in the NPls at𝑡 = 0are Poisson distributed within the range of the employed excitation
densities.^{123}The Poisson distribution function

𝑃(⟨𝑁 ⟩, 𝑁 ) = ⟨𝑁 ⟩^{𝑁}

𝑁 ! 𝑒^{−⟨𝑁 ⟩} (2.36)

reveals the probability for a NPl to contain𝑁excitons given a fixed value for⟨𝑁 ⟩(seeFigure 2.13). As
explained inSubsection 2.2.3, the ensemble of NPls contains a high number of individual elements
and therefore the law of large numbers may be considered, such that statistics apply to describe this
system. Then, the Poisson distribution𝑃(⟨𝑁 ⟩, 𝑁 )reflects the percentage of NPls containing𝑁excitons
as compared to the whole ensemble of𝑛_{total}NPls. Therefore,Equation 2.35can be rewritten as

𝑁total

∑

𝑁 =0

𝑃(⟨𝑁 ⟩, 𝑁 ) ⋅ 𝑛_{total}= 𝑛_{total}. (2.37)
For the sake of simplicity, in this thesis only the annihilation process𝑁 = 2to𝑁 = 1shall be compared
for different NPl thicknesses, i.e., the exciton-exciton annihilation lifetime𝜏_{2}shall be measured. To this
end, only measurements for which0.3 < ⟨𝑁 ⟩ < 0.4will be used for the analysis of this exciton-exciton
annihilation process. For values of⟨𝑁 ⟩in this range, around 4.3%of all NPls contain exactly two
excitons at𝑡 = 0, whereas only around 0.6%of all NPls contain more excitons than that, thereby
rendering this a good starting point for the determination of𝜏_{2}(seeFigure 2.13).

34 2.4 Dephasing